SUBMITTED TO: SUBMITTED BY:
DR. R.K. SAXENA ATUL RANJAN
J.D. Hwang, B.J. Li, W.S. Hwang, and C.T. Hu
(Submitted 8 December 1997; in revised form 5 March 1998)
Much effort recently has been expended to study the
strip casting process used to produce thin metal strip
with a near final thickness.
This process eliminates the need for hot rolling,
consumes less energy, and offer a feasible method of
producing various hard-to-shape alloys.
In this study strips of phosphor bronzes (Cu-Sn-P)
metal were produced using a twin roll strip casting
process as well as a conventional horizontal
continuous casting (HCC) process.
The results indicate that cast strip produced by a twin
roll caster exhibit significantly less inverse segregation
of tin compared to that produced by the HCC process.
The objective of the present study was to investigate the
major differences between phosphor bronze (C5191) sheet
produced using a horizontal twin roll caster and those
produced by the HCC process.
Strip with a width of 100 mm and thickness of 4.5 mm were
produced in a laboratory twin roll caster. Plate with much
larger dimensions (15 to 20 mm thick) produced by the
HCC process were obtained from a local mill.
Evaluation and analysis of the microstructures, macro
segregation, x-ray diffraction, and textures of the two types
of resulting materials were conducted.
Below Figure is a schematic diagram of the laboratory
horizontal twin roll caster used in the present study. Both
rolls are 400 mm in diameter, 100 mm in width, and are
made from a chromium copper alloy.
A horizontal nozzle was used to allow the molten metal to
flow into the caster in a smooth and non turbulent manner.
Surface quality of the cast strip was ensured by a stabilized
melt pool within the setback region during casting, which
can be achieved by maintaining a constant level of molten
metal inside the tundish.
SCHEMATIC OF THE HORIZONTAL
TWIN ROLL STRIP CASTER SYSTEM
ROLLING AND ANNEALING
PROCEDURES USED TO PRODUCE
THE TWIN ROLL CAST PHOSPHOR
A thicker plate (15.6 mm thick and 480 mm wide) of
phosphor bronze metal was fabricated with HCC
equipment in a local copper mill.
The HCC equipment consisted of high density graphite
molds, the inner surfaces of which were polished to reduce
Heat was extracted from the mold by a watercooled copper
The thickness of the cast plate was reduced to the final
gage of 0.2 to 0.5 mm after surface milling and a series of
cold rolling and annealing procedures.
MICRO CTRUCTURE OF PHOSPHOR
TWIN ROLL CASTING HCC
ANALYSIS OF MACROSEGREGATION
TWIN ROLL CASTING HCC
The present study demonstrates the technical advantages
of a new fabrication process—the twin roll strip casting—
for producing the phosphor bronze (C5191) alloy.
No inverse segregation is visible in the twin roll cast strip.
This can be attributed to the rapid casting speed and the
high cooling rate obtainable in this process.
The evidence presented suggests that solute enrichment of
tin in the central region of the twin roll cast strip is
responsible for the formation of fine equiaxed grains.
A significant difference exists between the two processes in
terms of preferred orientation in the as-cast condition.